##############################################################################
#                                                                            #
# This CIF contains the data in a paper accepted for publication in Acta     #
# Crystallographica Section B. It has been peer reviewed under the auspices  #
# of the IUCr Commission on Journals.                                        #
#                                                                            #
# Full details of the Crystallographic Information File format               #
# are given in the paper "The Crystallographic Information File (CIF):       #
# a New Standard Archive File for Crystallography" by S. R. Hall, F. H.      #
# Allen and I. D. Brown [Acta Cryst. (1991), A47, 655-685].                  #
#                                                                            #
# The current version of the core CIF dictionary may be obtained from        #
# ftp://ftp.iucr.org/pub/cif_core.dic. The current version number is 2.1.    #
#                                                                            #
# Software is freely available for graphical display of the structure(s) in  #
# this CIF.  For information consult the CIF home page http://www.iucr.org/  #
# cif/home.html                                                              #
#                                                                            #
#           Copyright International Union of Crystallography                 #
#                                                                            #
##############################################################################

data_innbte
_journal_data_validation_number     ?
_journal_date_recd_electronic     2001-03-29
_journal_date_accepted     2001-07-11
_journal_name_full     'Acta Crystallographica, Section B'
_journal_year     2001
_journal_volume     57
_journal_issue      5
_journal_page_first     665
_journal_page_last     672
_journal_paper_category     FA
_publ_contact_author_name
;
'Sander van Smaalen'
;
_publ_contact_author_address
;
Laboratory of Crystallography
University of Bayreuth
D-95440 Bayreuth
Germany
;
_publ_contact_author_email     smash@uni-bayreuth.de
_publ_contact_author_fax     '+49-921-55-3770'
_publ_contact_author_phone     '+49-921-55-3881'
_publ_section_title
;
Bulk modulus and non-uniform compression of Nb~3~Te~4 and In~x~Nb~3~Te~4
(x<1) channel compounds
;
loop_
    _publ_author_name
    _publ_author_address
    'Wunschel, Markus'
;       Laboratory of Crystallography
        University of Bayreuth
        D-95440 Bayreuth
        Germany
;
    'Dinnebier, Robert E.'
;       Laboratory of Crystallography
        University of Bayreuth
        D-95440 Bayreuth
        Germany
;
    'Carlson, Stefan'
;       MAX-Lab
        Lund University
        P.O. Box 118
        SE-22100 Lund
        Sweden
;
    'van Smaalen, Sander'
;       Laboratory of Crystallography
        University of Bayreuth
        D-95440 Bayreuth
        Germany
;
_chemical_name_systematic
;
?
;
_chemical_name_common     ?
_chemical_formula_moiety     'In0.54 Nb3 Te4'
_chemical_formula_sum     'In0.54 Nb3 Te4'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_weight     851.1
_chemical_melting_point     ?
_symmetry_cell_setting     hexagonal
_symmetry_space_group_name_H-M     'P 63/m'
loop_
    _symmetry_equiv_pos_site_id
    _symmetry_equiv_pos_as_xyz
    1 x,y,z
    2 x-y,x,1/2+z
    3 -y,x-y,z
    4 -x,-y,1/2+z
    5 -x+y,-x,z
    6 y,-x+y,1/2+z
    7 -x,-y,-z
    8 -x+y,-x,1/2-z
    9 y,-x+y,-z
    10 x,y,1/2-z
    11 x-y,x,-z
    12 -y,x-y,1/2-z
_cell_length_a     10.6768(3)
_cell_length_b     10.6768(3)
_cell_length_c     3.65660(10)
_cell_angle_alpha     90
_cell_angle_beta     90
_cell_angle_gamma     120
_cell_volume     360.99(2)
_cell_formula_units_Z     2
_cell_measurement_temperature     295
_cell_special_details
; ?
;
_exptl_absorpt_coefficient_mu     14.5
_exptl_absorpt_correction_type     none
_exptl_absorpt_process_details     ?
_exptl_absorpt_correction_T_min     ?
_exptl_absorpt_correction_T_max     ?
_exptl_special_details
; ?
;
_diffrn_ambient_temperature     295
_diffrn_radiation_type     synchrotron
_diffrn_radiation_wavelength      .13918
_diffrn_radiation_monochromator     ?
_diffrn_measurement_device_type     'ESRF ID15B'
_refine_special_details
; ?
;
_refine_ls_structure_factor_coef     Inet
_refine_ls_matrix_type     ?
_refine_ls_R_factor_all     ?
_refine_ls_goodness_of_fit_all     1.61
_refine_ls_restrained_S_all     ?
_refine_ls_restrained_S_obs     ?
_refine_ls_number_parameters     22
_refine_ls_number_restraints     ?
_refine_ls_number_constraints     ?
_refine_ls_hydrogen_treatment     ?
_refine_ls_weighting_scheme     ?
_refine_ls_weighting_details     ?
_refine_ls_shift/su_max     ?
_refine_ls_shift/su_mean     ?
_refine_ls_extinction_method     none
_refine_ls_extinction_coef     ?
loop_
    _atom_type_symbol
    _atom_type_scat_dispersion_real
    _atom_type_scat_dispersion_imag
    _atom_type_scat_source
    In  -.196  .475 International_Tables_Vol_C
    Nb  -.120  .234 International_Tables_Vol_C
    Te  -.246  .599 International_Tables_Vol_C
_computing_data_collection     ?
_computing_cell_refinement     'Jana2000'
_computing_data_reduction     'FIT2D'
_computing_structure_solution     ?
_computing_structure_refinement     'Jana2000'
_computing_molecular_graphics     ?
_computing_publication_material     ?
loop_
    _atom_site_label
    _atom_site_fract_x
    _atom_site_fract_y
    _atom_site_fract_z
    _atom_site_U_iso_or_equiv
    _atom_site_occupancy
    _atom_site_type_symbol
    Nb1  .4881(2)  .1024(2)  .25  .0054(3) 1 Nb
    Te2  .666667  .333333  .75  .0051(5) 1 Te
    Te3  .3356(2)  .271940(10)
                              .25  .0057(2) 1 Te
    In4 0 0 0  .028(3)  .2696(17) In
    In5 0 0  .25  .029(3)  .2696(17) In
_geom_special_details     ?
loop_
    _geom_bond_atom_site_label_1
    _geom_bond_atom_site_label_2
    _geom_bond_site_symmetry_1
    _geom_bond_site_symmetry_2
    _geom_bond_distance
    Nb1 Nb1 . 1_554 3.65660(10)
    Nb1 Nb1 . 1_556 3.65660(10)
    Nb1 Nb1 . 7_655 2.957(2)
    Nb1 Nb1 . 7_656 2.957(2)
    Nb1 Nb1 . 8_665 3.878(2)
    Nb1 Nb1 . 3_655 3.8777(18)
    Nb1 Te2 . 1_554 2.8905(10)
    Nb1 Te2 . . 2.8905(10)
    Nb1 Te3 . . 2.979(2)
    Nb1 Te3 . 3_655 2.792(2)
    Nb1 Te3 . 9_555 2.7790(12)
    Nb1 Te3 . 9_556 2.7790(12)
    Te2 Te2 . 1_554 3.65660(10)
    Te2 Te2 . 1_556 3.65660(10)
    Te2 Te3 . . 3.7346(15)
    Te2 Te3 . 1_556 3.7346(15)
    Te2 Te3 . 8_665 3.7346(11)
    Te2 Te3 . 8_666 3.7346(11)
    Te2 Te3 . 3_655 3.7346(19)
    Te2 Te3 . 3_656 3.7346(19)
    Te3 Te3 . 1_554 3.65660(10)
    Te3 Te3 . 1_556 3.65660(10)
    Te3 Te3 . 2_554 3.770(2)
    Te3 Te3 . 2_555 3.770(2)
    Te3 Te3 . 9_555 3.770(2)
    Te3 Te3 . 9_556 3.770(2)
    Te3 In4 . . 3.4209(11)
    Te3 In4 . 2_555 3.4209(11)
    Te3 In5 . . 3.2965(11)
    Te3 In5 . 7_555 3.7695(10)
    Te3 In5 . 7_556 3.7695(10)
    In4 In4 . 1_554 3.65660(10)
    In4 In4 . 1_556 3.65660(10)
    In4 In4 . 2_554 1.8283
    In4 In4 . 2_555 1.8283
    In4 In5 . 1_554 2.7425
    In4 In5 . .  .9142
    In4 In5 . 7_555  .9142
    In4 In5 . 7_556 2.7425
    In5 In5 . 1_554 3.65660(10)
    In5 In5 . 1_556 3.65660(10)
    In5 In5 . 7_555 1.8283
    In5 In5 . 7_556 1.8283
loop_
    _geom_angle_atom_site_label_1
    _geom_angle_atom_site_label_2
    _geom_angle_atom_site_label_3
    _geom_angle_site_symmetry_1
    _geom_angle_site_symmetry_3
    _geom_angle
    _geom_angle_publ_flag
    Nb1 Nb1 Nb1 1_554 1_556 180 .
    Nb1 Nb1 Nb1 1_554 7_655 51.81(3) .
    Nb1 Nb1 Nb1 1_554 7_656 128.19(6) .
    Nb1 Nb1 Nb1 1_554 8_665 90 .
    Nb1 Nb1 Nb1 1_554 3_655 90 .
    Nb1 Nb1 Te2 1_554 1_554 50.76(2) .
    Nb1 Nb1 Te2 1_554 . 129.24(4) .
    Nb1 Nb1 Te3 1_554 . 90 .
    Nb1 Nb1 Te3 1_554 3_655 90 .
    Nb1 Nb1 Te3 1_554 9_555 48.86(2) .
    Nb1 Nb1 Te3 1_554 9_556 131.14(4) .
    Nb1 Nb1 Nb1 1_556 1_554 180 .
    Nb1 Nb1 Nb1 1_556 7_655 128.19(6) .
    Nb1 Nb1 Nb1 1_556 7_656 51.81(3) .
    Nb1 Nb1 Nb1 1_556 8_665 90 .
    Nb1 Nb1 Nb1 1_556 3_655 90 .
    Nb1 Nb1 Te2 1_556 1_554 129.24(4) .
    Nb1 Nb1 Te2 1_556 . 50.76(2) .
    Nb1 Nb1 Te3 1_556 . 90 .
    Nb1 Nb1 Te3 1_556 3_655 90 .
    Nb1 Nb1 Te3 1_556 9_555 131.14(4) .
    Nb1 Nb1 Te3 1_556 9_556 48.86(2) .
    Nb1 Nb1 Nb1 7_655 1_554 51.81(3) .
    Nb1 Nb1 Nb1 7_655 1_556 128.19(6) .
    Nb1 Nb1 Nb1 7_655 7_656 76.38(5) .
    Nb1 Nb1 Nb1 7_655 8_665 136.37(3) .
    Nb1 Nb1 Nb1 7_655 3_655 95.55(5) .
    Nb1 Nb1 Te2 7_655 1_554 88.62(3) .
    Nb1 Nb1 Te2 7_655 . 139.29(7) .
    Nb1 Nb1 Te3 7_655 . 136.42(4) .
    Nb1 Nb1 Te3 7_655 3_655 57.73(5) .
    Nb1 Nb1 Te3 7_655 9_555 58.14(5) .
    Nb1 Nb1 Te3 7_655 9_556 106.61(6) .
    Nb1 Nb1 Nb1 7_656 1_554 128.19(6) .
    Nb1 Nb1 Nb1 7_656 1_556 51.81(3) .
    Nb1 Nb1 Nb1 7_656 7_655 76.38(5) .
    Nb1 Nb1 Nb1 7_656 8_665 136.37(3) .
    Nb1 Nb1 Nb1 7_656 3_655 95.55(5) .
    Nb1 Nb1 Te2 7_656 1_554 139.29(7) .
    Nb1 Nb1 Te2 7_656 . 88.62(3) .
    Nb1 Nb1 Te3 7_656 . 136.42(4) .
    Nb1 Nb1 Te3 7_656 3_655 57.73(5) .
    Nb1 Nb1 Te3 7_656 9_555 106.61(6) .
    Nb1 Nb1 Te3 7_656 9_556 58.14(5) .
    Nb1 Nb1 Nb1 8_665 1_554 90 .
    Nb1 Nb1 Nb1 8_665 1_556 90 .
    Nb1 Nb1 Nb1 8_665 7_655 136.37(3) .
    Nb1 Nb1 Nb1 8_665 7_656 136.37(3) .
    Nb1 Nb1 Nb1 8_665 3_655 60.00(5) .
    Nb1 Nb1 Te2 8_665 1_554 47.87(3) .
    Nb1 Nb1 Te2 8_665 . 47.87(3) .
    Nb1 Nb1 Te3 8_665 . 45.76(4) .
    Nb1 Nb1 Te3 8_665 3_655 109.86(6) .
    Nb1 Nb1 Te3 8_665 9_555 115.41(7) .
    Nb1 Nb1 Te3 8_665 9_556 115.41(7) .
    Nb1 Nb1 Nb1 3_655 1_554 90 .
    Nb1 Nb1 Nb1 3_655 1_556 90 .
    Nb1 Nb1 Nb1 3_655 7_655 95.55(5) .
    Nb1 Nb1 Nb1 3_655 7_656 95.55(5) .
    Nb1 Nb1 Nb1 3_655 8_665 60.00(5) .
    Nb1 Nb1 Te2 3_655 1_554 47.87(2) .
    Nb1 Nb1 Te2 3_655 . 47.87(2) .
    Nb1 Nb1 Te3 3_655 . 105.76(5) .
    Nb1 Nb1 Te3 3_655 3_655 49.86(5) .
    Nb1 Nb1 Te3 3_655 9_555 138.63(2) .
    Nb1 Nb1 Te3 3_655 9_556 138.63(2) .
    Te2 Nb1 Te2 1_554 . 78.47(3) .
    Te2 Nb1 Te3 1_554 . 79.02(4) .
    Te2 Nb1 Te3 1_554 3_655 82.16(4) .
    Te2 Nb1 Te3 1_554 9_555 96.39(2) .
    Te2 Nb1 Te3 1_554 9_556 160.67(9) .
    Te2 Nb1 Te2 . 1_554 78.47(3) .
    Te2 Nb1 Te3 . . 79.02(4) .
    Te2 Nb1 Te3 . 3_655 82.16(4) .
    Te2 Nb1 Te3 . 9_555 160.67(9) .
    Te2 Nb1 Te3 . 9_556 96.39(2) .
    Te3 Nb1 Te3 . 3_655 155.62(6) .
    Te3 Nb1 Te3 . 9_555 81.72(6) .
    Te3 Nb1 Te3 . 9_556 81.72(6) .
    Te3 Nb1 Te3 3_655 . 155.62(6) .
    Te3 Nb1 Te3 3_655 9_555 115.87(7) .
    Te3 Nb1 Te3 3_655 9_556 115.87(7) .
    Te3 Nb1 Te3 9_555 . 81.72(6) .
    Te3 Nb1 Te3 9_555 3_655 115.87(7) .
    Te3 Nb1 Te3 9_555 9_556 82.29(3) .
    Te3 Nb1 Te3 9_556 . 81.72(6) .
    Te3 Nb1 Te3 9_556 3_655 115.87(7) .
    Te3 Nb1 Te3 9_556 9_555 82.29(3) .
    Te2 Te2 Te2 1_554 1_556 180 .
    Te2 Te2 Te3 1_554 . 60.688(12) .
    Te2 Te2 Te3 1_554 1_556 119.312(12) .
    Te2 Te2 Te3 1_554 8_665 60.688(9) .
    Te2 Te2 Te3 1_554 8_666 119.312(9) .
    Te2 Te2 Te3 1_554 3_655 60.688(16) .
    Te2 Te2 Te3 1_554 3_656 119.312(16) .
    Te2 Te2 Te2 1_556 1_554 180 .
    Te2 Te2 Te3 1_556 . 119.312(12) .
    Te2 Te2 Te3 1_556 1_556 60.688(12) .
    Te2 Te2 Te3 1_556 8_665 119.312(9) .
    Te2 Te2 Te3 1_556 8_666 60.688(9) .
    Te2 Te2 Te3 1_556 3_655 119.312(16) .
    Te2 Te2 Te3 1_556 3_656 60.688(16) .
    Te3 Te2 Te3 . 1_556 58.624(17) .
    Te3 Te2 Te3 . 8_665 98.08(3) .
    Te3 Te2 Te3 . 8_666 128.30(4) .
    Te3 Te2 Te3 . 3_655 98.08(2) .
    Te3 Te2 Te3 . 3_656 128.30(2) .
    Te3 Te2 Te3 1_556 . 58.624(17) .
    Te3 Te2 Te3 1_556 8_665 128.30(4) .
    Te3 Te2 Te3 1_556 8_666 98.08(3) .
    Te3 Te2 Te3 1_556 3_655 128.30(2) .
    Te3 Te2 Te3 1_556 3_656 98.08(2) .
    Te3 Te2 Te3 8_665 . 98.08(3) .
    Te3 Te2 Te3 8_665 1_556 128.30(4) .
    Te3 Te2 Te3 8_665 8_666 58.624(13) .
    Te3 Te2 Te3 8_665 3_655 98.08(3) .
    Te3 Te2 Te3 8_665 3_656 128.30(3) .
    Te3 Te2 Te3 8_666 . 128.30(4) .
    Te3 Te2 Te3 8_666 1_556 98.08(3) .
    Te3 Te2 Te3 8_666 8_665 58.624(13) .
    Te3 Te2 Te3 8_666 3_655 128.30(3) .
    Te3 Te2 Te3 8_666 3_656 98.08(3) .
    Te3 Te2 Te3 3_655 . 98.08(2) .
    Te3 Te2 Te3 3_655 1_556 128.30(2) .
    Te3 Te2 Te3 3_655 8_665 98.08(3) .
    Te3 Te2 Te3 3_655 8_666 128.30(3) .
    Te3 Te2 Te3 3_655 3_656 58.62(2) .
    Te3 Te2 Te3 3_656 . 128.30(2) .
    Te3 Te2 Te3 3_656 1_556 98.08(2) .
    Te3 Te2 Te3 3_656 8_665 128.30(3) .
    Te3 Te2 Te3 3_656 8_666 98.08(3) .
    Te3 Te2 Te3 3_656 3_655 58.62(2) .
    Te3 Te3 Te3 1_554 1_556 180 .
    Te3 Te3 Te3 1_554 2_554 60.99(3) .
    Te3 Te3 Te3 1_554 2_555 119.01(5) .
    Te3 Te3 Te3 1_554 9_555 60.99(2) .
    Te3 Te3 Te3 1_554 9_556 119.01(4) .
    Te3 Te3 In4 1_554 . 74.50(2) .
    Te3 Te3 In4 1_554 2_555 105.50(2) .
    Te3 Te3 In5 1_554 . 90 .
    Te3 Te3 In5 1_554 7_555 60.99(2) .
    Te3 Te3 In5 1_554 7_556 119.01(3) .
    Te3 Te3 Te3 1_556 1_554 180 .
    Te3 Te3 Te3 1_556 2_554 119.01(5) .
    Te3 Te3 Te3 1_556 2_555 60.99(3) .
    Te3 Te3 Te3 1_556 9_555 119.01(4) .
    Te3 Te3 Te3 1_556 9_556 60.99(2) .
    Te3 Te3 In4 1_556 . 105.50(2) .
    Te3 Te3 In4 1_556 2_555 74.50(2) .
    Te3 Te3 In5 1_556 . 90 .
    Te3 Te3 In5 1_556 7_555 119.01(3) .
    Te3 Te3 In5 1_556 7_556 60.99(2) .
    Te3 Te3 Te3 2_554 1_554 60.99(3) .
    Te3 Te3 Te3 2_554 1_556 119.01(5) .
    Te3 Te3 Te3 2_554 2_555 58.03(3) .
    Te3 Te3 Te3 2_554 9_555 98.46(3) .
    Te3 Te3 Te3 2_554 9_556 128.14(4) .
    Te3 Te3 In4 2_554 . 56.57(3) .
    Te3 Te3 In4 2_554 2_555 73.04(3) .
    Te3 Te3 In5 2_554 . 64.07(3) .
    Te3 Te3 In5 2_554 7_555 51.86(2) .
    Te3 Te3 In5 2_554 7_556 81.54(3) .
    Te3 Te3 Te3 2_555 1_554 119.01(5) .
    Te3 Te3 Te3 2_555 1_556 60.99(3) .
    Te3 Te3 Te3 2_555 2_554 58.03(3) .
    Te3 Te3 Te3 2_555 9_555 128.14(4) .
    Te3 Te3 Te3 2_555 9_556 98.46(3) .
    Te3 Te3 In4 2_555 . 73.04(3) .
    Te3 Te3 In4 2_555 2_555 56.57(3) .
    Te3 Te3 In5 2_555 . 64.07(3) .
    Te3 Te3 In5 2_555 7_555 81.54(3) .
    Te3 Te3 In5 2_555 7_556 51.86(2) .
    Te3 Te3 Te3 9_555 1_554 60.99(2) .
    Te3 Te3 Te3 9_555 1_556 119.01(4) .
    Te3 Te3 Te3 9_555 2_554 98.46(3) .
    Te3 Te3 Te3 9_555 2_555 128.14(4) .
    Te3 Te3 Te3 9_555 9_556 58.03(3) .
    Te3 Te3 In4 9_555 . 56.57(2) .
    Te3 Te3 In4 9_555 2_555 73.04(2) .
    Te3 Te3 In5 9_555 . 64.07(2) .
    Te3 Te3 In5 9_555 7_555 51.86(2) .
    Te3 Te3 In5 9_555 7_556 81.54(2) .
    Te3 Te3 Te3 9_556 1_554 119.01(4) .
    Te3 Te3 Te3 9_556 1_556 60.99(2) .
    Te3 Te3 Te3 9_556 2_554 128.14(4) .
    Te3 Te3 Te3 9_556 2_555 98.46(3) .
    Te3 Te3 Te3 9_556 9_555 58.03(3) .
    Te3 Te3 In4 9_556 . 73.04(2) .
    Te3 Te3 In4 9_556 2_555 56.57(2) .
    Te3 Te3 In5 9_556 . 64.07(2) .
    Te3 Te3 In5 9_556 7_555 81.54(2) .
    Te3 Te3 In5 9_556 7_556 51.86(2) .
    In4 Te3 In4 . 2_555 30.998(10) .
    In4 Te3 In5 . . 15.499(5) .
    In4 Te3 In5 . 7_555 13.514(3) .
    In4 Te3 In5 . 7_556 44.512(13) .
    In4 Te3 In4 2_555 . 30.998(10) .
    In4 Te3 In5 2_555 . 15.499(5) .
    In4 Te3 In5 2_555 7_555 44.512(13) .
    In4 Te3 In5 2_555 7_556 13.514(3) .
    In5 Te3 In5 . 7_555 29.013(8) .
    In5 Te3 In5 . 7_556 29.013(8) .
    In5 Te3 In5 7_555 . 29.013(8) .
    In5 Te3 In5 7_555 7_556 58.026(16) .
    In5 Te3 In5 7_556 . 29.013(8) .
    In5 Te3 In5 7_556 7_555 58.026(16) .
    In4 In4 In4 1_554 1_556 180 .
    In4 In4 In4 1_554 2_554 0 .
    In4 In4 In4 1_554 2_555 180 .
    In4 In4 In5 1_554 1_554 0 .
    In4 In4 In5 1_554 . 180 .
    In4 In4 In5 1_554 7_555 0 .
    In4 In4 In5 1_554 7_556 180 .
    In4 In4 In4 1_556 1_554 180 .
    In4 In4 In4 1_556 2_554 180 .
    In4 In4 In4 1_556 2_555 0 .
    In4 In4 In5 1_556 1_554 180 .
    In4 In4 In5 1_556 . 0 .
    In4 In4 In5 1_556 7_555 180 .
    In4 In4 In5 1_556 7_556 0 .
    In4 In4 In4 2_554 1_554 0 .
    In4 In4 In4 2_554 1_556 180 .
    In4 In4 In4 2_554 2_555 180 .
    In4 In4 In5 2_554 1_554 0 .
    In4 In4 In5 2_554 . 180 .
    In4 In4 In5 2_554 7_555 0 .
    In4 In4 In5 2_554 7_556 180 .
    In4 In4 In4 2_555 1_554 180 .
    In4 In4 In4 2_555 1_556 0 .
    In4 In4 In4 2_555 2_554 180 .
    In4 In4 In5 2_555 1_554 180 .
    In4 In4 In5 2_555 . 0 .
    In4 In4 In5 2_555 7_555 180 .
    In4 In4 In5 2_555 7_556 0 .
    In5 In4 In5 1_554 . 180 .
    In5 In4 In5 1_554 7_555 0 .
    In5 In4 In5 1_554 7_556 180 .
    In5 In4 In5 . 1_554 180 .
    In5 In4 In5 . 7_555 180 .
    In5 In4 In5 . 7_556 0 .
    In5 In4 In5 7_555 1_554 0 .
    In5 In4 In5 7_555 . 180 .
    In5 In4 In5 7_555 7_556 180 .
    In5 In4 In5 7_556 1_554 180 .
    In5 In4 In5 7_556 . 0 .
    In5 In4 In5 7_556 7_555 180 .
    In5 In5 In5 1_554 1_556 180 .
    In5 In5 In5 1_554 7_555 0 .
    In5 In5 In5 1_554 7_556 180 .
    In5 In5 In5 1_556 1_554 180 .
    In5 In5 In5 1_556 7_555 180 .
    In5 In5 In5 1_556 7_556 0 .
    In5 In5 In5 7_555 1_554 0 .
    In5 In5 In5 7_555 1_556 180 .
    In5 In5 In5 7_555 7_556 180 .
    In5 In5 In5 7_556 1_554 180 .
    In5 In5 In5 7_556 1_556 0 .
    In5 In5 In5 7_556 7_555 180 .
